Carbon nanomaterial Formation on Fresh-Reduced Iron by Converted Natural Gas
© The Author(s). 2017
Received: 18 January 2017
Accepted: 31 January 2017
Published: 10 February 2017
The mechanism of carbon nanomaterial formation at moderate temperatures while processing fresh-reduced iron by products of air conversion of natural gas is considered. It is shown that under given conditions, the size and the shape of the resulting carbon are dependent on the temperature and the size of microscopic iron grains formed during reduction. These iron grains are the catalyzer of the reaction of carbon monoxide disproportionation. It is concluded that the formation of a nucleus of the new carbon phase occurs at the contact boundaries of neighboring grains of newly reduced iron with the subsequent formation in these places of ring-shaped carbon cuffs. Nanotubes are forming as a result of further carbon crystallization, and separation of iron particles from the main mass is occurring, i.e., there is a fragmentation of the substance of the catalyst. According to the results of laboratory studies, the optimum temperature of carbon nanotube formation in the environment of converted gas is 600–650 °C. The evidence of the hypothesis that the mechanism of the reaction of carbon monoxide disproportionation flows through the intermediate stage of iron oxides formation is given.
Recirculated throat (waste) gases are typically used for cooling the product produced in shaft furnaces of direct iron reduction . In these circumstances, the process of carbon formation is released. This carbon is formed from carbon monoxide contained in the waste gases. It is known  that the fresh-reduced iron is a catalyst in the decomposition reaction of carbon monoxide, while its decomposition in a pure gas environment at atmospheric pressure is practically not observed.
However, further studies showed that while chemisorption of the CO molecule on the catalyst occurs, weakening of the bond between carbon and oxygen atoms occurs very slowly. This fact suggests that the mechanism of carbon formation is unlikely .
Carbon may be formed, depending on the conditions, widely differing between each other flake form or in the form of carbon nanotubes, nanofibers, and in a special conditions, in a form of fullerenes  or diamonds .
Results and Discussion
Based on the analysis of literature and data of laboratory studies [10, 11], the mechanism of CNTs formation in the area of moderate temperature (up to 700 °C) in a general form can be represented as follows.
where V oxide and V metal are, accordingly, the volumes of oxide and metal formed from it after reduction; A metal and M oxide are the atomic weight of the metal and the molecular weight of its oxide; ρ metal and ρ oxide are the density of the metal and its oxide; and n is the number of metal atoms in the molecule of its oxide.
i.e., the volume of iron (III) oxide at its reduction becomes smaller more than two times. A highly dispersed structure of iron in the form of chaotic piles of separate grains is formed as a result of restructuring of the crystal lattice and decrease of the catalyst volume. Further, this phenomenon has a considerable influence on the formation of the resulting carbon material.
As a result, the material gets a developed surface  and consists of small variously oriented crystals of iron, a lattice of which contains many defects. Iron atoms have increased activity because of noncompensated chemical bonds, a manifestation of iron ignitibility. Boundaries are formed of a type of “insular Motta model” between touching grains of the metal . Order in the arrangement of atoms could largely be absent on the boundary of grain contact according to this model. Such boundaries are called incoherent.
It is known  that the largest number of defects in the crystal lattice of iron is on incoherent boundaries of contact of the grains, contacting with each other. These areas have high catalytic activity. The release of carbon atoms first of all occurs at the process of CO decomposition with a subsequent formation of nuclei of a new solid phase. The emergence of a new phase at the grain boundaries also contributes to a higher diffusion rate of carbon atoms in these locations [15, 16]. Located on the surface of the crystal lattice of the iron atoms, in contrast to that which is situated inside due to noncompensated chemical bonds between them, a force field is created . The effect of these fields is enhanced at the points of contact of contiguous iron grains. They presumably also contribute to the catalytic activity of these places and the emergence of a new phase.
Prior to carbon phase formation, the induction period exists during which there is an accumulation of free carbon atoms with the increase of their concentration up to a critical value at which the beginning of a new phase formation occurs. Study on thermogravimetric installation shows that the induction period at a temperature of 650 °C is about 8–10 min.
The resulting carbon cuff provides for a wedging effect on grains of a metal, and as a result of a subsequent deposition (crystallization) of carbon atoms (at constant outer and inner diameters of the cuff), the separation of grains from the main “mainland” part of the catalyst occurs (Fig. 3b). Thus, the fragmentation of the grains of iron at the initial stage of the formation of carbon nanotubes occurs after dispersion of the catalyst metal at the phase of metal reduction. It should be noted that stresses occurring during carbon crystallization can reach large values. As the results show cases of destruction of iron ore pellets, masonry of blast furnaces in the environment of CO-containing gases have a place in practice.
The atoms of carbon formed on various active centers of the surface of a separated catalyst particle, due to the existing concentration gradient, diffuse toward the board of contact of the particles with the nanotube, where their crystallization occurs. The growth of nanotube primarily oriented along the line connecting the centers of contacting catalyst grains. Because grains are mainly randomly located, growth of nanotubes occurs in different directions relative to the wafer surface coated by a catalyst. In addition, the catalyst activity in different areas of the separated iron particle is not identical and therefore carbon deposition rate at different points along the line of particle contact with the growing nanotube varies; this leads to curvature of the latter. Apparently, mechanical interaction of the tubes with each other at the process of their growth also contributes to curvature. As a result, the material looks like “tangled hair.”
At a temperature of 923 K (650 °C), the maximum solubility of carbon in iron is only 0.013%. Taking into the consideration the low solubility of carbon, the migration of its atoms from active centers to the place of CNTs growth, for our opinion, is mainly due to the surface diffusion, especially that its speed by 2–3 orders is higher than internal . This is also evidenced by the fact that the formed nanofibers are hollow inside. Indeed, the delivery of carbon atoms into the internal part of the fibers presupposes their diffusion through the crystal lattice of iron, i.e., internal diffusion.
The formation of ferrite and cementite (Fe3C) with polymorphic transformation of γ-Fe → α-Fe in the steel is the evidence of the insufficiently high internal diffusion capacity of carbon. Despite the fact that formation of graphite is energetically more favorable, the decomposition of austenite at low temperatures usually occurs with a pearlite formation , due to the relatively slow speed of diffusion of carbon atoms in iron. Apparently, carbon atoms in its crystal lattice have a mutual repulsion that does not accelerate carbon internal diffusion .
As can be seen from Fig. 6, reactions (5) and (6) become thermodynamically impossible in the temperature region exceeding 700 °C. According to the experimental data, CNTs formation in this field also is terminated.
It is obvious that the higher the content of hydrogen in the source gas, reactions (10) and (11) will run in more degrees compared with (7) and (8). This raises the proportion of carbon which forms according to the final gross reaction (12) in comparison with reaction (9) that was confirmed in the experiment .
The following experimentally observed fact is evidenced in a favor of an assumption about the possibility of iron oxides forming in the present conditions. In the case when the substrate for the catalyst is a plate of transformer steel, the formation of the carbon material (in any form) is suppressed. It is known that the transformer steel contains a high content of silica (up to 4.5% ). Silicon has a high affinity for oxygen, so even a slight presence in the gas phase of oxidants CO2 and H2O leads to its oxidation .
Apparently, the formed silicon oxide reacts with iron oxide (II) appearing on the active centers with the formation of chemical compounds of fayalite—Fe2SiO4. Negative value of isobaric potential of fayalite formation (line 3, Fig. 6) is evidence of the thermodynamic possibility of its formation, the data is borrowed from . As a result, catalyst deactivation occurs and carbon formation is not observed. Paper  indicates observations in practice cases of carbon and iron oxides formation at low temperature in an environment with a high ratio of CO/CO2 during steel annealing in heat-treatment furnaces. Finally, iron oxides are detected in the X-ray pictures of iron catalyst samples after pre-reduction by hydrogen, and then processing by mixture of carbon monoxide with nitrogen .
Emitted carbon at temperatures above 700 °C has a scaly structure. While at lower temperatures, it is synthesized in the form of nanotubes. This fact suggests that in the temperature range below 700 °C, cycles of oxidation-reduction of iron catalyst play a crucial role in the process of CNTs formation. This factor, together with the inextricable relation to the process of carbon emissions by the reactions (5) and (6) contributes to the fragmentation of iron into tiny particles smaller than 300 nm and ultimately nanotube formation. At temperatures above 700 °C, decomposition of carbon monoxide occurs on another mechanism without the stage of iron oxides formation. In this case, although there is a fragmentation of the catalyst, the forming iron particles are larger and emitting carbon has a scaly shape.
It is noteworthy that the visible surface of iron particles is close to spherical under the form. Special studies  showed that even at room temperature, crystals of various metals under the action of surface tension forces change their form in the direction of reducing their external surface. However, at low temperatures, this process proceeds very slowly and becomes noticeable only after a long time (several months). Spheroidization of iron particles proceeds much faster at temperatures of CNTs formation and microscopic size of iron particles. Apparently, many times, repeating cycles of iron oxidation-reduction also plays a big role in the process of spheroidization which leads to a weakening of the bonds between the atoms in the crystal lattice and thereby contributes for intensification of their self-diffusion.
The mechanism of occurrence and growth of CNTs on iron catalyst under conditions of low-temperature disproportionation of carbon monoxide contained in products of air conversion of natural gas is considered.
A highly dispersed structure of iron in the form of a chaotic accumulation of its particles of microscopic size is formed In terms of low-temperature reduction, the boundaries of contact of particles have the highest catalytic activity, where the nucleation of a new phase occurs in the form of ring-shaped cuffs due to emitted carbon while carbon monoxide decomposes. Fragmentation of the catalyst with separation of iron particles from the main mass occurs as the result of carbon subsequent crystallization. The outer diameter of nanotubes formed while growth of carbon cuffs is determined by the size of separated iron particles. The optimum temperature for CNTs formation from products of air conversion of natural gas is 600–650 °C. It was suggested that the mechanism of carbon nanotube formation in considered conditions flows through the intermediate stage of oxidation-reduction of iron on the active centers of the catalyst.
This work was supported by the State Fund for Fundamental Research of Ukraine (contract F64-35).
AN and DF carried out the experiments, data processing, and preparation and approval of the final manuscript. VK and AS contributed to the statement of the problem and the way to solve it. AK discussed the results and helped prepare and approve the final manuscript. BB contributed to the statement of the problem and discussion of the results. All authors read and approved the final manuscript.
The authors declare that they have no competing interests.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
- Bondarenko BI, Shapovalov VA, Garmash NI. Teorija i tehnologija beskoksovoj metallurgii. – Kiev: Nauk. Dumka. 2003.Google Scholar
- Pod red. Rojtera VA. Kataliticheskie svojstva veshhestv. Spravochnik. Kiev, Naukovadumka. 1968.Google Scholar
- Rostovcev ST. Teorija metallurgicheskih processov. M.: Metallurgizdat. 1956.Google Scholar
- Esin OA, Gel’d PV (1962) Fizicheskaja himija pirometallurgicheskih processov. Sverdlovsk, MetallurgizdatGoogle Scholar
- Kolesnik NF, Kudievskij SS, Kirichenko AG, Priluckij OV. Termokataliticheskij raspad monooksida ugleroda. Zaporozh’e: Izdatel’stvo Zaporozhskoj gosudarstvennoj inzhenernoj akademii. 2006.Google Scholar
- Chesnokov VV, Bujanov RL. Obrazovanie uglerodnyh nitej pri kataliticheskom razlozhenii uglevodorodov na metallah podgruppy zheleza i ih splavah. Uspehi himii, Tom 69, №7, 2000; 675 – 692.Google Scholar
- Pod red. Gnesina GG, Skorohoda VV. Neorganicheskoe materialovedenie. Osnovy nauki o materialah. T. 1. Kiev, Naukovadumka; 2008.Google Scholar
- Derjagin BV, Fedoseev DV. Rost almaza i grafita iz gazovoj fazy. M.: Nauka, 1977.Google Scholar
- Messerle VE, Ustimenko AB (2013) Plazmennaja pererabotka uglej. Teplojenergetika 12:23–29Google Scholar
- Bondarenko B, Sviatenko O, Kotov V, Khovavko A, Filonenko D, Nebesniy A, Vishnevsky A (2013) Research of the technology of carbon nanotubes production in gas mixtures contained CO. International Journal of Energy for a Clean Environment 14(2–3):177–182. doi:10.1615/InterJEnerCleanEnv2014006802 View ArticleGoogle Scholar
- Alexander Khovavko, Alexey Sviatenko, Viktor Kotov, Borys Bondarenko, Andriy Nebesniy, Denis Filonenko Technology of carbon nanotubes in gas mixtures containing carbon monoxide. Physica Status Solidi. 2013; doi: 10.1002/pssc.201200971.Google Scholar
- Uvarova IV. Fenomenologicheskie aspekty dispergirovanija produktov pri topohimicheskih reakcijah vosstanovlenija metallov iz oksidov (obzor). Poroshkovaja metallurgija, №2, 1990. – p. 59 – 65.Google Scholar
- Livshic BG. Metallografija. – M.: Metallurgija, Izd. 2-e, ispr. i dop. 1971; 405.Google Scholar
- Guljaev AP. Metallovedenie. – M.: Metallurgija, 1978. – 647 p.Google Scholar
- Pod red. Kana R. Fizicheskoe metallovedenie. Vyp. 2. Fazovye prevrashhenija. Metallografija. Per. s angl. – M: Mir, 1968. – 490 p.Google Scholar
- Bokshtejn BS, Bokshtejn SZ, Zhuhovickij AA. Termodinamika i kinetika diffuzii v tverdyh telah. – M.: Metallurgija, 1974; 280.Google Scholar
- Dzhejkok M, Parfit Dzh. Himija poverhnostej razdela faz. – M.: Mir, 1984. – 269 p.Google Scholar
- Korotich V. Osnovy teorii i tehnologii podgotovki syr’ja k domennoj plavke. – M.: Metallurgija, 1978; 208.Google Scholar
- Harris P. Uglerodnye nanotruby i rodstvennye struktury. Novye materialy XXI veka. – M.: Tehnosfera, 2003; 336.Google Scholar
- Pikunov MV, Desipri AI Metallovedenie. – M: Metallurgija, 1980; 256.Google Scholar
- Kurdjumov GV, Utevskij LM Jentin RI. Prevrashhenie v zheleze i stali. – M.: Nauka, 1977; 238.Google Scholar
- Krishtal MA. Mehanizm diffuzii v zheleznyh splavah. – M.: Metallurgija, 1972; 399.Google Scholar
- Vladimirov LP. Termodinamicheskie raschety ravnovesija metallurgicheskih reakcij. – M.: Metallurgija, 1970; 528.Google Scholar
- Kotov VG, Svyatenko AM, Khovavko AI, Nebesnyi AA, Filonenko DS. Jeksperimental’nye issledovanija processa sazheobrazovanija pri vysokoj koncentracii vodoroda v gaze, soderzhashhem monooksid ugleroda. Jenergotehnologii i resursosberezhenie. 2014; № 2; 33–38.Google Scholar
- Dubrov NF, Lapkin NI. Jelektrotehnicheskie stali. – M: Metallurgija. 1963; 384.Google Scholar
- Vashhenko AI, Zen’kovskij AG. Okislenie i obezuglerozhivanie stali. M: Metallurgija. 1972;336.Google Scholar
- Bogdandi L, Jengel’ G.Ju. Vosstanovlenie zheleznyh rud. M: Metallurgija. 1971; 520.Google Scholar
- Jestrin BM. Proizvodstvo i primenenie kontroliruemyh atmosfer. – M.: Metallurgija, 1973; 392.Google Scholar
- Naumov VA, Pavlova TN. Issledovanie kinetiki reakcii disproporcionirovanija okisi ugleroda na zheleznom katalizatore. ZhFH, №6, 1972. – p. 1480 – 1483.Google Scholar
- Ivensen VA. Fenomenologija spekanija i nekotorye voprosy teorii. M.: Metallurgija. 1985; 246.Google Scholar